Litharge

== Description ==
A heavy yellow powder composed of lead monoxide. Litharge is prepared as the oxidized product of molten lead that has been stirred or atomized to incorporate air then cooled and ground to form the yellow powder. Massicot, another crystalline form of lead monoxide, occurs naturally but can also be made by heating lead carbonate to 300C. Litharge is lightly more orange than massicot due to some formation of red lead oxide. Both forms of lead monoxide has been used as a drier in oil and as a low-fire [[flux] in making ceramics and glass. They were used as a yellow pigments in paints and glazes. Thin layers of lead monoxide are used to produce iridescent colors on brass and bronze. It has also been used as a filler for rubber and to produce artificial tortoiseshell and horn. Litharge is mixed with glycerol to make plumber's cement.
== Synonyms and Related Terms ==
massicot; lead monoxide; lithargyros (Gr.); plumbum ustum (Latin); Lithargit (Deut.); Massicot (Deut.); litharge (Fr.); litargirio (Esp.); litargirio (giallo di piombo) (It.); massicot (Ned.); litharge (Ned.); litargírio (Port.); yellow lead oxide; plumbous oxide
[[[SliderGallery rightalign|Litharge (284).TIF~FTIR (MFA)|Litharge (Forbes MFA 284) (640x445).jpg~Raman (MFA)|PIG284.jpg~XRD|f284sem.jpg~SEM|f284edsbw.jpg~EDS|Slide30 FC284.PNG~XRF]]]
== Risks ==
* Toxic by inhalation or ingestion. 
* Skin contact may cause irritation or ulcers. 
* Carcinogen, teratogen, suspected mutagen. 
* ThermoFisher: SDS
==Physical and Chemical Properties==
Soluble in acetic acid, dilute nitric acid and alkalis. Insoluble in water and ethanol. Turns gray on exposure to sulfur fumes.
In transmitted PPL, the tetragonal alpha-PbO (the beta-PbO referring to massicot) form translucent particles ranging in color from pale yellow and pale yellow-orange to pale green. Some semi-opaque particles of dark reddish-brown color are also reported. Most particles are rounded in shape and other reported morphologies include square, rectangular and acicular shapes. Particles tend to agglomerate into clumps. Relief is very high and RI is greater than 1.662. 
In transmitted XPL, the particles are highly birefringent with third-order jewel tones. Extinction is straight, but clumps of particles will not show complete extinction and appear to 'twinkle' as the stage is rotated. Clumps of particles display a strong yellow body color, and smaller particles may exhibit a dull yellowish outline at extinction. Acicular particles are length-fast. 
Composition 	PbO
CAS 	1317-36-8
Melting Point 	888 C
Density 	9.40-9.53 g/ml
Refractive Index	2.51; 2.71; 2.61
== Additional Images ==
File:Litharge PPL 400x.jpg|Litharge, PPL 400x
File:Litharge XPL2 400.jpg|Litharge, XPL 400x
File:Litharge, squarish particle, PPL 1000x.jpg|Litharge particle with squarish morphology, PPL 1000X
File:Litharge, squarish particle at extinction, PPL 1000x.jpg|Litharge particle with squarish morphology at extinction, XPL 1000X
File:Litharge, squarish particle at brightest point, PPL 1000x.jpg|Litharge particle with squarish morphology at brightest point, XPL 1000X
== Resources and Citations ==
* Eastaugh, N., et. al. "The Pigment Compendium: a Dictionary and Optical Microscopy of Historical Pigments", Butterworth-Heinemann, London, 2008
* R. J. Gettens, G.L. Stout, Painting Materials, A Short Encyclopaedia, Dover Publications, New York, 1966 Comment: density 9.40 and ref. index 2.51; 2.71; 2.61
* Thomas Gregory, The Condensed Chemical Dictionary, Reinhold Publishing, New York, 3rd ed., 1942
* Ralph Mayer, A Dictionary of Art Terms and Techniques, Harper and Row Publishers, New York, 1969 (also 1945 printing)
* Susan E. Schur, Conservation Terminology: A review of Past & Current Nomenclature of Materials, Technology and Conservation, Spring (p.34-39); Summer (p.35-38); Fall (p.25-36), 1985
* Dictionary of Building Preservation, Ward Bucher, ed., John Wiley & Sons, Inc., New York City, 1996
Category:Materials database